Sorption behaviour in a unique 3,12-connected zinc‒organic framework with 2.4 nm cages
Qian, Jinjie; Jiang, Feilong; Su, Kongzhao; Pan, Jie; Zhang, Linjie; Li, Xingjun; Yuan, Daqiang; Hong, Maochun; Journal of Materials Chemistry A 1 (2013) 10631–; doi:10.1039/c3ta12391j

data_7239544
_publ_section_title
;
 Sorption behaviour in a unique 3,12-connected zinc--organic framework
 with 2.4 nm cages
;
_journal_issue                   36
_journal_name_full               'Journal of Materials Chemistry A'
_journal_page_first              10631
_journal_paper_doi               10.1039/c3ta12391j
_journal_volume                  1
_journal_year                    2013
_chemical_formula_sum            'C11 H5 N0.5 O3 Zn0.75'
_chemical_formula_weight         241.18
_space_group_IT_number           204
_space_group_name_Hall           '-I 2 2 3'
_space_group_name_H-M_alt        'I m -3'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'I m -3'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            48
_cell_length_a                   27.3685(2)
_cell_length_b                   27.3685(2)
_cell_length_c                   27.3685(2)
_cell_measurement_reflns_used    13499
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      72.8220
_cell_measurement_theta_min      3.9270
_cell_volume                     20500.0(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_detector_area_resol_mean 5.2797
_diffrn_measured_fraction_theta_full 0.966
_diffrn_measured_fraction_theta_max 0.966
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_source         'SuperNova (Cu) X-ray Source'
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0190
_diffrn_reflns_av_sigmaI/netI    0.0110
_diffrn_reflns_limit_h_max       32
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            16467
_diffrn_reflns_theta_full        67.39
_diffrn_reflns_theta_max         67.39
_diffrn_reflns_theta_min         3.96
_exptl_absorpt_coefficient_mu    1.571
_exptl_absorpt_correction_T_max  0.9256
_exptl_absorpt_correction_T_min  0.8846
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    0.938
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             5808
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.05
_platon_squeeze_details
;
;
_refine_diff_density_max         1.674
_refine_diff_density_min         -1.905
_refine_diff_density_rms         0.102
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.086
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     162
_refine_ls_number_reflns         3190
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.092
_refine_ls_R_factor_all          0.0841
_refine_ls_R_factor_gt           0.0799
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1863P)^2^+29.2467P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2435
_refine_ls_wR_factor_ref         0.2527
_reflns_number_gt                2820
_reflns_number_total             3190
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ta12391j.txt
_cod_data_source_block           FJI-2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_symmetry_cell_setting' value 'Cubic' was changed to
'cubic' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_exptl_crystal_density_meas' value 'not measured' was
changed to '?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_sg_symbol_H-M      Im-3
_cod_original_formula_sum        'C11 H5 N0.50 O3 Zn0.75'
_cod_database_code               7239544